Extraction of Palladium(II) and Platinum(IV) from Hydrochloric Acid Solutions with Trioctylammonium Nitrate Ionic Liquid without Dilution
- 30 Downloads
The fundamental properties and extraction capability of an ionic liquid (IL), trioctylammonium nitrate ([HTOA][NO3]), for PdII and PtIV, are investigated. At room temperature, [HTOA][NO3] is a solid (melting point: 30.7 °C), but it becomes a liquid (melting point: 16.7 °C) when saturated with water. Water-saturated [HTOA][NO3] exhibits a viscosity of 267.1 mPa·s and an aqueous solubility of 2.821 × 10−4 mol·dm−3 at 25 °C, and can be used as an extraction solvent without dilution. [HTOA][NO3] exhibits an extremely high extraction capability for PdII and PtIV in dilute hydrochloric acid (0.1–2 mol·dm−3 HCl); the distribution ratio reaches 3 × 104 for both the metals. From electrospray ionization mass spectrometry analysis, the species extracted in the IL phase are [PdCl3]− and [PdCl2(NO3)]− for PdII and [PtCl6]2− and [PtCl5]− for PtIV. A majority of the other transition metals are considerably less or marginally extracted into [HTOA][NO3] from a 0.1 mol·dm−3 hydrochloric acid solution. The extraction capacity of [HTOA][NO3] is greater than that of other hydrophobic ILs such as [HTOA]Cl and bis(trifluoromethanesulfonyl)imide-based ILs. The metals extracted into the IL phase are quantitatively back-extracted using an aqueous solution containing thiourea and nitric acid. By controlling the thiourea concentration and shaking time, PdII and PtIV are mutually separated to some extent in the back extraction process. The IL phase used for the back extraction can be reused for the forward extraction of these metals after scrubbing it with an aqueous nitric acid solution.
KeywordIonic liquid Water-saturated trioctylammonium nitrate Extraction Palladium(II) Platinum(IV)
The authors thank Ms. Sayaka Kado (Center for Analytical Instrumentation, Chiba University) for her technical support on mass spectrometry. The authors also thank Enago (www.enago.jp) for the English language review. This work was financially supported by JSPS KAKENHI Grant Number JP26410145.
- 1.PGM Market Report May 2017. Johnson Matthey Precious Metals Management, Royston (2017)Google Scholar
- 2.Fornalczyk, A., Saternus, M.: Removal of platinum group metals from the used auto catalytic converters. Metalurgija 48, 133–136 (2009)Google Scholar
- 4.Cox, M.: Solvent extraction in hydrometallurgy. In: Rydberg, J., Cox, M., Musikas, C., Choppin, G.R. (eds.) Solvent Extraction Principles and Practice, 2nd edn, pp. 454–503. CRC/Taylor and Francis, Boca Raton (2004)Google Scholar
- 5.De Los Rios, A.P., Hernandez-Fernandez, F.J. (eds.): Ionic Liquids in Separation Technology. Elsevier, Amsterdam (2014)Google Scholar
- 33.Kasahara, I., Kanai, M., Taniguchi, M., Kakeba, A., Hata, N., Taguchi, S., Goto, K.: Bis[2-(5-bromo-2-pyridylazo)-5-(N-propyl-N-sulphopropylamino)phenolato]cobaltate(III) as a counter ion for the extraction and spectrophotometric determination of long-chain quaternary ammonium salts and tertiary alkylamines in the presence of each other. Anal. Chim. Acta 219, 239–245 (1989)CrossRefGoogle Scholar
- 38.Riddick, J.A., Bunger, W.B., Sakano, T.K.: Organic Solvents, 4th edn. Wiley, New York (1986)Google Scholar
- 39.Högfeldt, E. (ed.): Stability Constants of Metal-Ion Complexes Part A: Inorganic Ligands. Pergamon Press, Oxford (1982)Google Scholar
- 40.Kondo, K., Ourachi, T., Kaneiwa, T., Matsumoto, M.: Solvent extraction of precious metals with quaternary ammonium salts and its application to preparation of metal particles. Solvent Extr. Res. Dev. Jpn. 7, 176–184 (2000)Google Scholar